Polymorphism of CaTeO~3~ and solid solutions Ca~<i>x~</i>Sr~1{-~<i>x</i>}TeO~3~
Stöger, Berthold; Weil, Matthias; Zobetz, Erich; Giester, Gerald; Acta Crystallographica Section B 65 (2009) 167–181; doi:10.1107/S0108768109002997

data_2104342
_publ_section_title
;
 Polymorphism of CaTeO~3~ and solid solutions
 Ca~<i>x~</i>Sr~1{-~<i>x</i>}TeO~3~
;
_journal_coeditor_code           SN5078
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              167
_journal_page_last               181
_journal_paper_doi               10.1107/S0108768109002997
_journal_volume                  65
_journal_year                    2009
_chemical_formula_structural     'Ca Te O3'
_chemical_formula_sum            'Ca O3 Te'
_chemical_formula_weight         215.68
_chemical_name_systematic
;
 calcium(II) tellurium(IV) oxide - beta prime
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                108.604(9)
_cell_angle_beta                 112.393(13)
_cell_angle_gamma                32.3190(10)
_cell_formula_units_Z            18
_cell_length_a                   25.6215(5)
_cell_length_b                   10.3933(2)
_cell_length_c                   11.2481(2)
_cell_measurement_reflns_used    25213
_cell_measurement_temperature    275(2)
_cell_measurement_theta_max      36.24
_cell_measurement_theta_min      2.07
_cell_volume                     1480.59(16)
_computing_cell_refinement       'Denzo (Otwinowski & Minor, 1997)'
_computing_data_collection       'Collect (Nonius, 1998)'
_computing_data_reduction        'Denzo (Otwinowski & Minor, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      275(2)
_diffrn_measured_fraction_theta_full 0.944
_diffrn_measured_fraction_theta_max 0.944
_diffrn_measurement_device_type  'Nonius Kappa-CCD'
_diffrn_measurement_method       \w-scans
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0466
_diffrn_reflns_av_sigmaI/netI    0.0687
_diffrn_reflns_limit_h_max       40
_diffrn_reflns_limit_h_min       -41
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            25213
_diffrn_reflns_theta_full        36.24
_diffrn_reflns_theta_max         36.24
_diffrn_reflns_theta_min         2.07
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    10.391
_exptl_absorpt_correction_T_max  0.7812
_exptl_absorpt_correction_T_min  0.3686
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'HKL-Scalepack (Otwinowsky & Minor, 2003)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    4.354
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       fragment
_exptl_crystal_F_000             1728
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.03
_refine_diff_density_max         2.402
_refine_diff_density_min         -2.116
_refine_ls_extinction_coef       0.00085(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.013
_refine_ls_matrix_type           full
_refine_ls_number_parameters     407
_refine_ls_number_reflns         13485
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.013
_refine_ls_R_factor_all          0.0623
_refine_ls_R_factor_gt           0.0344
_refine_ls_shift/su_max          0.004
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0210P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0606
_refine_ls_wR_factor_ref         0.0679
_reflns_number_gt                10052
_reflns_number_total             13485
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn5078.cif
_cod_data_source_block           bprime-CaTeO3-275
_cod_original_cell_volume        1480.59(5)
_cod_database_code               2104342
_cod_database_fobs_code          2104342